### Mechanics of fragmentation of crocodile

### skin and other thin films

Zhao Qin1,2_{, Nicola M. Pugno}3,4,5_{& Markus J. Buehler}1,2,6

1_{Laboratory for Atomistic and Molecular Mechanics (LAMM), Department of Civil and Environmental Engineering, Massachusetts}
Institute of Technology, 77 Massachusetts Ave., Room 1-239, Cambridge 02139, MA, USA,2_{Center for Computational}
Engineering, Massachusetts Institute of Technology, 77 Massachusetts Ave., Cambridge, MA 02139, USA,3_{Laboratory of}
Bio-Inspired & Graphene Nanomechanics, Department of Civil, Environmental and Mechanical Engineering, Universita` di Trento,
via Mesiano, 77 I-38123 Trento, Italy,4_{Center for Materials and Microsystems, Fondazione Bruno Kessler, Via Sommarive 18,}
38123 Povo (Trento),5_{School of Engineering & Materials Science, Queen Mary University of London, Mile End Road, London E1}
4NS, UK,6_{Center for Materials Science and Engineering, Massachusetts Institute of Technology, 77 Massachusetts Ave.,}
Cambridge, MA 02139, USA.

Fragmentation of thin layers of materials is mediated by a network of cracks on its surface. It is commonly seen in dehydrated paintings or asphalt pavements and even in graphene or other two-dimensional materials, but is also observed in the characteristic polygonal pattern on a crocodile’s head. Here, we build a simple mechanical model of a thin film and investigate the generation and development of fragmentation patterns as the material is exposed to various modes of deformation. We find that the characteristic size of fragmentation, defined by the mean diameter of polygons, is strictly governed by mechanical properties of the film material. Our result demonstrates that skin fragmentation on the head of crocodiles is dominated by that it features a small ratio between the fracture energy and Young’s modulus, and the patterns agree well with experimental observations. Understanding this mechanics-driven process could be applied to improve the lifetime and reliability of thin film coatings by mimicking crocodile skin.

## S

kin fragmentation (also known as crocodile cracking), is a common way for thin films to release deforma-tion energy that is caused by tension1–3_{. This process is irreversible and leaves complex pattern as many}

cracks interact and go through the material surface. The geometry and size of those fragmentation patterns
varies dramatically for different materials including organic and inorganic systems such as fruit skin, paintings
and ceramics4,5_{, as well as a nanofilm with atomic thickness}6_{(Fig. 1). They are generally considered a threat to}

engineering systems. For instance, steel and wood structures in buildings and turbines with fragmented coating materials are largely exposed to environment and subjected to corrosion. It is critical to understand the mech-anism behind such phenomena crossing multiple scales. Especially, how tensile forces initiate the fragmentation in thin films and what material characteristic stabilizes the pattern remain largely illusive. Fundamental answer-ing of those questions can help the design of surface coatanswer-ing with improved lifetime and resistance.

The fragmented skin on a crocodile’s head provides a suitable case to investigate the skin fragmentation. The
skin acts like scales of snakes, lizards and fishes7,8_{to protect the crocodile, but instead of gene regulation, its}
pattern is induced by skeletal growth during the embryonic stage9_{. This contradicts with the conventional}
thinking, suggesting that some fragmentation may actually enhance the protection function. Moreover, it is
intriguing, but unclear, what is the mechanical basis for crocodiles to generate this skin fragmentation with a
characteristic size. By learning from the fragmentation of crocodile skin, we expect to gain knowledge in
improv-ing the design of engineered surface coatimprov-ings.

In our current study, we combine theoretical analysis with numerical simulation that uses a simple thin film
model for the crocodile skin. We note that prior studies have investigated the fragmentation in surface coatings
using numerical methods, but most of them require pre-existing defects for crack initiation10–13_{. It is difficult to}
decouple the effect of random distributions of weak regions and the effect of material property on the
character-istic of fragmentation pattern by using those models. Here, we use a simple elastic network model with a uniform
spring stiffness and strength (detail in the Methods section), without additional defects, to investigate how the
characteristic size of fragmentation is affected by mechanical properties of the film material and loading
condi-tions. It is shown that by adjusting the spring characteristic we can reproduce the characteristic of fragmentation
pattern as is found in different materials including crocodile skin.

SUBJECT AREAS: COARSE-GRAINED MODELS BIOPHYSICS MECHANICAL ENGINEERING Received 2 October 2013 Accepted 19 March 2014 Published 27 May 2014 Correspondence and requests for materials should be addressed to M.J.B. (mbuehler@ MIT.EDU)

Results

Here we use a simple network model to study the fragmentation behavior of the thin film as depicted schematically in Fig. 1g (details see Methods section). We apply biaxial tensile strain to this model to investigate how fragmentation generates and grows. The fragmenta-tion pattern is identified as an assembly of polygons as shown in Fig. 2a. Notably, cracking only appears beyond a critical level of deformation (denoted by the strain ef, where strain is defined as the length increase divided by the initial length), as shown in Figs. 2b. The deformation in the material decreases for strain beyond efby creating more fragments and decreasing their sizes. We measure the average fragment size as a function of strain as shown in Fig. 2c (detail in Methods section). It is shown that for strain beyond efthe fragmentation size keeps decreasing, until it reaches a secondary critical deformation state (denoted by the strain ec) when the pattern becomes stabilized and strain increases exclusively, leading to further opening the already-cracked edges of polygons. This results in an asymptotic fragment size. Using fracture mechanics theory, we

derive how such fragmentation follows deformation by relating the deformation energy in the material to the surface energy used to create cracks (details see Methods section). We find that the frag-ment size during stretching can be expressed by:

L~L?z

4c 1{vð Þ az1ð Þ ﬃﬃﬃ

3 p

Eeðaz1Þ for e§ef ð1Þ where E is the material’s Young’s modulus, n is Poisson’s ratio, 2c is the fracture energy per unit area of the material, e is the applied tensile strain caused by the mismatch between thin film and sub-strate, L‘is the length of the residue scale, which is the asymptotic size and a is the stiffening factor that relates to the nonlinear material property of skin (detail in the Methods section). From this equation, we find that the evolution of the fragment size is governed by two factors: the applied strain as well as the ratio between the fracture energy and the material stiffness. The comparison of the importance of those two factors is adjusted by the nonlinearity given by a. We summarize some plausible values for 2c/E for different skins (human hand, chicken and crocodile) measured in experiments as shown in Table 1. Those values are used to fit the simulation result as shown in Fig. 2c. We find that only small 2c/E value, as is observed in crocodile skin, gives a good interpretation for the simulation result. From this analysis we also obtain the empirical value of a as 2.4, which corre-sponds to a stiffening hyper-elastic material, as common in nature. Moreover, we find the best fit with unphysical negative L‘values for human hand and chicken, while physical positive L‘ value for a crocodile. This result suggests that it is the mechanical force and releasing of deformation energy that dominates the fragmentation of crocodile skin and makes the pattern eventually reach the stable characteristic length of L‘(Fig. 1a). The negative L‘value, in con-trast, suggests the surface geometry of those skins is not caused by fragmentation, as they can form corrugated pattern with more com-plex geometry but not asymptotic size (until the cellular size) (as shown in Fig. 1c).

We change the mechanical characteristic of the network structure
(changing from a 5 2.4 to a 5 1 and 7) by using different power
exponent of the constituent springs and compare the characteristic
nature of the fragmentation in those different systems, as shown in
Fig. 3. It is seen that the fragmentation starts to appear in the linear
elastic material (a 5 1) at a smaller strain (ef50.05) than the
hyper-elastic material and the hyper-hyper-elastic material with strong
strain-stiffening characteristic (a 5 7) generate the fragmentation at a much
larger strain (Fig. 3b). Moreover, for a 5 7, it is observed that the
fragmentation starts with many disconnected small cracks as shown
in Fig. 3a, suggesting that this strain-stiffening material is able to
diffuse the deformation energy in the entire deformed region instead
of concentrating at several crack tips14_{. Further increasing the}
deformation for this material quickly lead to the fragmentation
pat-tern with many small fragments (L 5 0.2 cm as shown in Fig. 3b).
We measure each fragment length of the three materials (a 5 1, 2.4
and 7) at the end of simulation of e 5 0.2 and obtain the probability
distribution as shown in Fig. 3c. It is found that both a 5 1 and 7 lead
to smaller fragments with more uniform (Lmax/L 5 1.9 and 1.8, for a
51 and 7, respectively, where Lmaxis the maximum length and L is
the average length of all the fragments) and symmetric distribution of
the fragment length than a 5 2.4 which contains fragments much
larger than the rest (Lmax/L 5 2.5). The result obtained for a 5 1
quantitatively agrees with the experimental observation for oxide
coating, which is taken as a linear-elastic material, as Lmax/L 5
1.65 , 1.8 is obtained for this material under different applied
strains12_{. These results agree with what we observe for crocodile skin}
and other thin films (Fig. 1) as the fragments in crocodile skin
(Fig. 1a) are larger and have more irregular length than in
linear-elastic material (ceramics and surface coating in Figs. 1f and b,
respectively) or hyper-elastic material with strong strain-stiffening

Figure 1|Widely observed skin fragmentation patterns in animals, paint, skin, food, plants and ceramics. (a), Snapshot of a crocodile head. Bottom: close-up of skin fragmentation in the form of scales on a crocodile head surface (the crocodile is small with an eye to nose distance of 90 mm). Scale bar: 4 mm [Boston, MA, image credit to ZQ]. (b), Skin fragmentation observed on the surface of painted door [Boston, MA, image credit to ZQ]. Scale bar: 1 cm. (c), Skin crumpling observed on the back of a hand. Scale bar: 2 mm [Boston, MA, image credit to ZQ]. (d), Skin fragmentation observed on cookie surface. Scale bar: 16 mm [Boston, MA, image credit to ZQ]. (e), Skin fragmentation pattern observed on a cantaloupe surface. Scale bar: 6 mm [Boston, MA, image credit to ZQ]. (f), Skin fragmentation observed on the inner surface of a porcelain cup [Boston, MA, image credit to ZQ]. Scale bar: 3 mm. (g), Schematic of the mechanical model used to model skin fragmentation under deformation. The overarching question for those phenomena is how tensile forces initiate the fragmentation and what material characteristic determines the geometry of the patterns as we observe on different surfaces.

characteristic (human skin in Fig. 1c), suggesting again that the fragmentation pattern of crocodile skin is strictly governed by its mechanical properties.

We now change the strain rate and investigate how the
deforma-tion speed alters the fragmentadeforma-tion pattern. The stabilized patterns
under multiple strain rates are as shown in Fig. 4a, where it is
demon-strated that a faster strain rate induces more fragments with smaller
size. The asymptotic size of polygons L‘, as systematically shown in
Fig. 4b, more clearly illustrates that the fragmentation is strongly
rate-dependent at small deformation rate while becomes insensitive
of large deformation rate. By considering—as posed by classical
vis-coelasticity—the scaling E(t) , E(t 5 0)/(t/t 1 1) (t is
a characteristic time)15_{, since e~}

ð

_e tð Þdt~_et where t is the time for applying deformation of constant strain rate, assuming the asymptotic size is proportional to the fragment size at largest strain we obtain that L?!c

Eeaz1_{max}

!_e{1zconst (here emax.ecis the applied strain for obtaining asymptotic fragment size). This relation-ship is used to fit the simulation results as shown in Fig. 3b. Indeed, this mechanism, combined with the anisotropic growth of the head skull, explains the anisotropic and irregular fragmentation pattern seen in crocodiles (Figs. 5h and i). This result also suggests that the fragmentation pattern varies for paints because of the different deforming history caused by environmental change, generating the unique fingerprint on each of them. It is also noted that for small

loading rate, the fragment size approximates exponential scaling, but the size departs from the exponential at larger loading rate because the resolution of the network structure for generating the fragments is limited by the initial length of the springs in the model, which has the physical meaning of the size of the constituent particles such as cellular size of the skin. This factor can be involved by combining experimental measurements of cellular size to improve the biological insight of the model in future.

We systematically compare the simulation result against in situ
observations of the fragmentation of crocodile head, as illustrated in
Fig. 5. It is clearly seen that the emerging fragmentation pattern very
well reproduce what is observed on the crocodile head. The
connec-tivity of the polygons has an average value of 3.03 to 3.21 (with and
without boundary), and this connectivity range yields a mean
num-ber of sides of polygons between 5.88 and 5.31. This is in excellent
agreement with the experimental observation of 5.532 ref. [9], and
indicates that polygons are nearly hexagonal and those closer to the
boundary have more sides. Moreover, the model shows that
intro-ducing heterogeneous deformation—considering that the strain rate
(or bone growth) in one direction is faster than that in the other,
orthogonal direction–captures the characteristic laddering shape on
the top of crocodile’s head as illustrated in Figs. 5h and i. This finding
demonstrates that the laddering scale pattern observed on crocodile
head is caused by the fact that the head’s longitudinal growth is faster
than in other directions9,16_{. To demonstrate the significance of the}

Figure 2|Illustration of the process of fragmentation under biaxial tensile deformation. (a), The increasing strain leads to evolving cracking
patterns in different stages; (I) no crack, (II) crack growth, (III) forming a stationary network of cracks, and (IV) further opening of existing cracks
without newly formed cracks. (b), The overall strain-stress relation during deformation, with the four stages shown in (a) marked on the graph. (c), The
increasing strain leads to growing fragments with decreased size, yielding an asymptotic size of L‘when the material is fully fractured (i.e. stage IV
depicted in a) and no further changes in fragmentation pattern are induced by strain increments. The continuum curves are fitted according to Eq. (3) by
using 2c/E 5 3 3 1021_{, 4 3 10}22_{and 2 3 10}24_{cm for human hand skin, chicken skin and crocodile skin (finding a 5 2.4), respectively. The typical}

Poisson’s ratio, n 5 1/3, is used here. The agreement between the simulation result and the fitted curve based on the mechanics of crocodile skin suggests that the asymptotic size of fragmentation is dominated by the small ratio between the fracture toughness and stiffness.

Table 1 | Fracture energy (2c) and Young’s modulus (E) of skin of different animals

Skin type Fracture energy (2c) (kJ/m2_{)} _{Young’s modulus (E) (MPa)} _{Ratio (2c/E) (m)}

Human hand skin [19,32] 1.8 0.6 0.003

Chicken skin [33] 2.8 8 0.0004

fragmentation of crocodile, we summarize the connectivity of the fragmentation pattern of different systems as shown in Fig. 6. It is shown that the fragmentation of crocodile head has similar geometry as is observed in cantaloupe, ceramics and paint and their patterns are all captured by our mechanics model. The significant difference for the skin crumpling of hand skin indicates that the corrugated pattern with complex geometry is governed by involving other mechanisms rather than tension-induced fragmentation.

Discussion

In this study, we identify two critical strains (ef for initiating of
fragmentation and ecfor reaching the asymptotic fragment size),
which are induced by skeletal growth, that govern the initial and
final mechanics of skin fragmentation. Those two critical strains
divide the deformation procedure into three regimes, which agrees
with what is observed in the cracking of other thin film systems17_{,}
except that our results do not statistically depend on the initial
ran-dom distribution of defects. The first critical strain explains why
there is no fragments found before 45 days of embryonic crocodile,
as is found by in situ observation9_{, likely because the accumulated}
strain remains below the threshold (ef) during that period. The
sec-ond critical strain explains why the pattern does not change (or
re-develop anew) repeatedly over time, as no new polygons are created
by the increasing strain above the other threshold (ec). Our result also
shows that the fragmentation depends on the ratio between the
frac-ture energy and Young’s modulus of the skin. The mechanical
prop-erty of crocodile skin makes it unique to form the polygon pattern
during development. Flexible skins of other animals, such as
mam-mal and bird, are hard to reach a stable fragmentation pattern in the
skin under normal state. However, there are extreme conditions18_{, for}

Figure 3|Fragmentation under biaxial tensile deformation for two materials with different nonlinearity. (a), The simulation snapshots of evolving cracking pattern in linear elastic (a 5 1) material that is deformed at e 5 0.1 (I) and e 5 0.2 (II), and in hyper-elastic material (a 5 7) with strong stiffening behavior that is deformed at e 5 0.1 (III) and e 5 0.2 (IV). All the loading conditions are same as what is used in Fig. 2 but the fragmentation patterns are significant different. (b), The fragment size as function of the increasing strain for the elastic two materials (a 5 1 and 7). Data points I , IV correspond to the snapshot in a. It is shown that the fragmentation starts to appear in the linear elastic material at a strain (ef50.05) smaller than the hyper-elastic material (a 5 7 and 2.4 here and Fig. 2c, respectively). The hyper-elastic material with strong stiffening behavior (a 5 7), once generates fragmentation at a larger strain, quickly forms a pattern with many small fragments (L 5 0.2 cm). (c), The probability distribution (p) of fragment size measured from simulation snapshots of the three materials (a 5 1, 2.4 and 7) at the end of simulation of e 5 0.2. Both a 5 1 and 7 (1.0 6 0.3 and 0.25 6 0.1 cm, respectively) lead to more uniform and symmetric distribution of the fragment length than a 5 2.4 (1.8 6 1.1 cm) which contents some fragments much larger than the rest.

Figure 4|Illustration of the rate-dependent geometry under biaxial tensile deformation. (a), Snapshots of fragmentation patterns under different strain rates (I) slow, (II) medium, (III) fast. (b), Asymptotic size of polygons (L‘), when the material is fully fractured, as a function of the strain rate (_e), clearly showing a strain rate effect on the resulting pattern of the fragmentation geometry. The continuum curve is fitted according to L?!_e{1zconst. The result shows that the asymptotic size of

fragmentation depends on the strain rate, which implies the fragmentation pattern is tunable according to the loading conditions.

example dehydration, oldness and illness19–22_{, which can alter the}
mechanics of the skin and make the stable fragmentation possible.
From a different angle of view, the skin fragmentation of crocodile
can be attributed to mechanical adaption23_{. The hard skin of }
cro-codile with fragmentation can greatly increase the flexibility (with
reduced bending stiffness because cracks set fragments free-by
reduced entropic elasticity24_{-to move out of plane) and reduce the}
difficulty for movements at the end of jaw. A similar strategy is also
observed to be adopted by armoured fish as its discrete scales for
body protection and mobility20,25_{.}

The fragmentation on crocodile heads is unique for animal skins but shows a similar geometry as many inorganic thin films. Here, we investigated the mechanism hidden behind these phenomena by introducing a mechanical model and probing the entire fragmentation process. Our results demonstrate that the ratio between the fracture energy and Young’s modulus together with deformation rate governs the characteristic size of the fragmentation pattern. By using this knowledge learnt from crocodile skin, we may design and produce surface coating with improved stability by using synthetic materials. For instance, we may use heterogeneous distribution of stiff and soft materials, which mimic the crocodile scales and their joints, for coat-ing under the help of digital manufacturcoat-ing technologies. By uscoat-ing the strategies one can make the coating stable from further fragmentation and hence have longer lifetime and provide more efficient protection.

Methods

Details of the elastic network model.The model we use to simulate the fragmentation
behavior of keratinized epidermal under biaxial tension is a simple elastic network
model. The model is composed of a collection of beads and inter-bead connections
ref. [14,26]. The initial coordinates of all the beads are randomly distributed. The
topology of the inter-bead connection is designed by Delaunay triangulation
algorithm27_{. This method enables generating triangle meshwork from randomly}

distributed point and maximizes the minimum angle of all the angles of the triangles, avoiding irregular triangles. For each inter-bead connection in the triangulation, we use a breakable nonlinear springs to represent the interaction. The tensile force for each spring is given by f 5 dk0(Dr/r0)awhere r0is the initial length of the spring, Dr is the deformation of the spring, k0is the stiffness of a unit length spring, a is the stiffening factor that relates to the nonlinear property of the spring, d is a cut off function with its value given by d~ exp Dr

r0 {eb J z1 {1

with J~300 as the smooth factor
and eb50.05 as the bond breaking strain. It is noted that by using this force function,
the stiffness of each spring stochastically varies with its initial length, ensuring the
uniform mechanics of the material. Without loss of generality, all parameters in the
model, including bead mass, spring stiffness and film length are set unitless (without
any fitting). We apply biaxial tensile strain to deform the entire film with an overall
constant strain rates. Yet the deformation is applied in a discrete from: for every a
hundred steps, we add the constant strains to the film at the first step and equilibrate
the film during the rest steps with the single layer of beads at the four edges fixed. This
loading method mimics the tension field caused by skeletal growth and applied on the
epidermal on the crocodile head as illustrated in Fig. 1g (considering that the bone is 1–
2 orders of magnitude stiffer than the epidermal and it can be modeled as a rigid
substrate to generate homogenous deformation to the epidermal in every single
direction28_{). This model enables us to systematically investigate how growth history}

and growth rate are coupled29_{to determine the evolution of fragmentation pattern.}

Figure 5|Comparison between the simulated fragmentation in a thin film andin situ observation of a crocodile’s head9_{. (a), Branching of the crack}

predicted in simulation. (b), Branching of the crack of in situ observation. (c), merging of two cracks based on simulation of two sequencing time steps.
(d), merging of two cracks of in situ observation. (e), The extension of a crack meets other cracks perpendicularly in simulation. (f), The extension of a
crack meets other cracks perpendicularly of in situ observation. (g), Probability distribution (P) of vertices as a function of connectivity, which denotes the
number of cracks connecting at each vertex, for polygons of the cracking pattern in simulation as the result for all polygons (red with square) and the result
without boundary polygons (blue with circle). Average values are indicated by dash lines. (h), The laddering pattern induced by heterogeneous strain rates
in simulation. (i), The laddering pattern of in situ observation on the top of crocodile’s head. All in situ observation images (b), (d), (f), (i) are reproduced
from9_{. The geometry of crocodile’s head scales shows similar characteristic as what is seen in the simulation, suggesting that our model captures the}

Monitoring fragmentation and computing its size in the simulation.During the post-analysis of the simulation we monitor the fragmentation pattern as assemblies of polygons by identifying all rupture springs (Dr/r0$0.05) and highlight them by taking snapshots. To compute the size of those polygons, we simply assume the cracks are in form of hexagonal lattices and the total lattice area is given by Atot~3

ﬃﬃﬃ 3 p

L2_{n}_{8}
where n is the number of scales and L/2 is length of the hexagonal edge (L is the scale
size), while the area of the polygon edge with width r0(the average spring length at
equilibrium) is Aedge~3Lr0n=2. Noting that the ratio between the area of the polygon
edge and total surface area equals the ratio between the number of beads involved in
broken bonds (Ncrackas a function of strain) and the total bead number (N). These
relations enable us to obtain the fragment size according to

L~4 ﬃﬃﬃ 3 p r0N 3Ncrack ð2Þ We have measured the distribution of fragment size for cases a 5 1, 2.4 and 7 and summarized the result in Fig. 3c. It is shown that the average value and standard deviation of the fragment is 1.0 6 0.3, 1.8 6 1.1 and 0.25 6 0.1 cm for a 5 1, 2.4 and 7 respectively, which agrees with the measurement given by using Eq. 2 as 0.8, 1.2 and 0.2 cm for a 5 1, 2.4 and 7, respectively as shown in Figs. 2c and 3b.

Fracture mechanics analysis for the fragmentation size.Here we derive how
fragmentation size follows deformation. The energy balance during crack
propagation imposes that the variation of the total potential energy dP, equal to the
variation of the elastic strain energy dW minus the variation of the external work dY,
must be equal to the opposite of the work spent in creating the new surface of
fragments dS, i.e dP 5 dW 2 dY 5 22cdS, where 2c is the fracture energy per unit
area. Assuming linearity for the constitutive law of the film implies the validity of the
Clapeyron’s theorem30_{, i.e. dW 5 dY/2. Accordingly, dP 5 2dW and the condition}

for fragmentation becomes dW 5 2cdS. Note that this result is in general valid also for
nonlinear systems under imposed displacements; for this case, in fact, the external
work is identically zero and thus we do not need to apply the Clapeyron’s theorem to
obtain it. By integration, we have DW 5 2cDS, where DS is the new crack surface area
created as DS 5 3/2nLb (for hexagonal fragmentation geometry) where n is the
number of scales, b is their thickness and L is their size. We now generalize the
stress-strain relation as s 5 Eea_{by considering the nonlinearity of materials and estimate the}

deformation energy as DW 5 2AbEe(a11)_{/(12n)/(a 1 1), where e is the accumulated}

mismatch biaxial strain between skin and skeleton, A is the film surface area, b is its thickness, E is the secant modulus that equals to Young’s modulus of linear material or general materials at small deformation, n is Poisson’s ratio and a is the stiffening factor that relates to the nonlinear material property of skin (a , 1 for elastic-plastic,

a 5 1 for linear, a . 1 for hyper-elastic material). Accordingly, the fragmentation is expected when the following system holds:

2 A{Að ?ÞEeðaz1Þ 1{v ð Þ az1ð Þ ½ ~3cnL e§ef ( ð3Þ where efis the skin fracture strain as shown in computational modelling and A‘is the residue area that still subjects to deformation after fragmentation that we assume to be proportional to the fragment perimeter where the residual deformations

concentrate31_{. Accordingly, since for the hexagonal geometry L}2~ 8A
3pﬃﬃﬃ3n, we can
define LL?~8A?

3pﬃﬃﬃ3nand the fragment size during stretching is given by Eq. (1). 1. Leterrier, Y., Boogh, L., Andersons, J. & Manson, J. A. E. Adhesion of silicon oxide

layers on poly(ethylene terephthalate) 1. Effect of substrate properties on coating’s fragmentation process. J. Polym. Sci., Part B: Polym. Phys. 35, 1449–1461 (1997). 2. Buehler, M. J. & Xu, Z. P. MATERIALS SCIENCE Mind the helical crack. Nature

464, 42–43 (2010).

3. Goehring, L., Conroy, R., Akhter, A., Clegg, W. J. & Routh, A. F. Evolution of mud-crack patterns during repeated drying cycles. Soft Matter 6, 3562–3567 (2010). 4. Leterrier, Y. et al. Biaxial fragmentation of thin silicon oxide coatings on

poly(ethylene terephthalate). Journal of Materials Science 36, 2213–2225 (2001). 5. Espinosa, H. D., Zavattieri, P. D. & Dwivedi, S. K. A finite deformation continuum

discrete model for the description of fragmentation and damage in brittle materials. J. Mech. Phys. Solids 46, 1909–1942 (1998).

6. Feng, X., Maier, S. & Salmeron, M. Water splits epitaxial graphene and intercalates. J. Am. Chem. Soc. 134, 5662–5668 (2012).

7. Chang, C. et al. Reptile scale paradigm: Evo-Devo, pattern formation and regeneration. Int. J. Dev. Biol. 53, 813–826 (2009).

8. Meyers, M. A., Lin, Y. S., Olevsky, E. A. & Chen, P. Y. Battle in the Amazon: Arapaima versus Piranha. Adv. Eng. Mater. 14, B279–B288 (2012).

9. Milinkovitch, M. C. et al. Crocodile Head Scales Are Not Developmental Units But Emerge from Physical Cracking. Science 339, 78–81 (2013).

10. Hornig, T., Sokolov, I. M. & Blumen, A. Patterns and scaling in surface fragmentation processes. Phys. Rev. E 54, 4293–4298 (1996).

11. Gao, S., Nakasa, K. & Kato, M. Analysis and simulation of cracking patterns in coating under biaxial tensile or thermal stress using analysis/FEM strain-accommodation method. Eng. Fract. Mech. 70, 1573–1591 (2003).

12. Andersons, J. & Leterrier, Y. Advanced fragmentation stage of oxide coating on polymer substrate under biaxial tension. Thin Solid Films 471, 209–217 (2005). 13. Meakin, P. A Simple-Model for Elastic Fracture in Thin-Films. Thin Solid Films

151, 165–190 (1987).

14. Qin, Z. & Buehler, M. J. Flaw Tolerance of Nuclear Intermediate Filament Lamina under Extreme Mechanical Deformation. Acs Nano 5, 3034–3042 (2011). 15. Piccardo, M., Chateauminois, A., Fretigny, C., Pugno, N. M. & Sitti, M. Contact

compliance effects in the frictional response of bioinspired fibrillar adhesives. J. R. Soc. Interface 10, 20130182 (2013).

16. Fukuda, Y., Saalfeld, K., Lindner, G. & Nichols, T. Estimation of Total Length from Head Length of Saltwater Crocodiles (Crocodylus porosus) in the Northern Territory, Australia. J. Herpetol. 47, 34–40 (2013).

17. Crosby, K. M. & Bradley, R. M. Fragmentation of thin films bonded to solid substrates: Simulations and a mean-field theory. Phys. Rev. E 55, 6084–6091 (1997).

18. Buehler, M. J. & Yung, Y. C. Deformation and failure of protein materials in physiologically extreme conditions and disease. Nat. Mater. 8, 175–188 (2009). 19. Agache, P. G., Monneur, C., Leveque, J. L. & De Rigal, J. Mechanical properties and

Young’s modulus of human skin in vivo. Arch. Dermatol. Res. 269, 221–232 (1980).

20. Yang, W. et al. Natural Flexible Dermal Armor. Adv. Mater. 25, 31–48 (2013). 21. Escoffier, C. et al. Age-related mechanical properties of human skin: an in vivo

study. J. Invest. Dermatol. 93, 353–357 (1989).

22. Loeys, B. L. et al. Mutations in fibrillin-1 cause congenital scleroderma: stiff skin syndrome. Sci. Transl. Med. 2, 23ra20 (2010).

23. Bock, W. J. The Definition and Recognition of Biological Adaptation. Am. Zool. 20, 217–227 (1980).

24. Verdier, P. H. Relaxation Behavior of the Freely Jointed Chain. J. Chem. Phys. 52, 5512–5517 (1970).

25. Bruet, B. J. F., Song, J., Boyce, M. C. & Ortiz, C. Materials design principles of ancient fish armour. Nat. Mater. 7, 748–756 (2008).

26. Qin, Z. & Buehler, M. J. Impact tolerance in mussel thread networks by heterogeneous material distribution. Nature Communications 4, 2187 (2013). 27. Lin, M. & Manocha, D. Applied Computational Geometry Towards Geometric

Engineering (Springer Berlin Heidelberg, 1996).

28. Bertram, J. E. A. & Gosline, J. M. Functional Design of Horse Hoof Keratin - the Modulation of Mechanical-Properties through Hydration Effects. J. Exp. Biol. 130, 121–136 (1987).

29. Cornetti, P., Pugno, N., Carpinteri, A. & Taylor, D. Finite fracture mechanics: A coupled stress and energy failure criterion. Eng. Fract. Mech. 73, 2021–2033 (2006).

30. Freund, L. B. Dynamic fracture mechanics. (CUP, Cambridge, 1990).

Figure 6|Comparison of the connectivity of the fragmentation patterns of different systems. Average values are given by main bars and the standard deviations are given by error bars. The simulation result is extracted from Fig. 4g without boundary polygons and its mean value and standard deviation are highlighted by dash lines. The agreement of the connectivity observed in simulation and other systems including crocodile, cantaloupe, ceramics and paint. The connectivity of hand skin shows significant different value. This result suggests that the mechanism revealed by our model explains the fragmentation of thin films on several different systems, while it does not account for generating the pattern on hand skin (perhaps because active cellular processes are involved).

31. Qin, Z. & Buehler, M. J. Cooperativity governs the size and structure of biological interfaces. J Biomech 45, 2778–2783 (2012).

32. Pereira, B. P., Lucas, P. W. & SweeHin, T. Ranking the fracture toughness of thin mammalian soft tissues using the scissors cutting test. J. Biomech. 30, 91–94 (1997).

33. Mahvash, M. et al. Modeling the forces of cutting with scissors. IEEE T. Bio-med. Eng. 55, 848–856 (2008).

34. McKittrick, J. et al. The Structure, Functions, and Mechanical Properties of Keratin. JOM-J. Min. Met. Mat. S. 64, 449–468 (2012).

Acknowledgments

Z.Q. and M.J.B. acknowledge support by NSF, ONR and AFOSR. N.M.P. is supported by the European Research Council with the following grants: ERC StG Bihsnam, ERC PoC Replica2 and ERC PoC Knotouth as well as by the European Union, within the Graphene Flagship.

Author contributions

Z.Q., N.M.P. and M.J.B. designed the research. Z.Q. implemented the computational model and analysis tools, carried out the simulations and collected the data. N.M.P. and Z.Q. performed the theoretical analysis and collected the data. Z.Q., N.M.P. and M.J.B. analyzed the results and wrote the paper.

Additional information

Competing financial interests:The authors declare no competing financial interests. How to cite this article:Qin, Z., Pugno, N.M. & Buehler, M.J. Mechanics of fragmentation of crocodile skin and other thin films. Sci. Rep. 4, 4966; DOI:10.1038/srep04966 (2014).

This work is licensed under a Creative Commons Attribution 3.0 Unported License. The images in this article are included in the article’s Creative Commons license, unless indicated otherwise in the image credit; if the image is not included under the Creative Commons license, users will need to obtain permission from the license holder in order to reproduce the image. To view a copy of this license, visit http://creativecommons.org/licenses/by/3.0/